COTTON FIBRE LENGTH EVALUATION:

Mean length.

Upper quartile.

Effective length.

Modal length.

2.5% span length.

50% span length.

It is that value of fibre length for which 3/4 of all the observed values in whole representative sample are lower, and 1/4 of all the observed value in whole representative sample are higher.

It is very difficult to define effective length technically. “ The upper quartile of a numerical length which is determined by making an arbitrary construction of a representative simple. This upper quartile length is called effective length of fibres”. In this arbitrary construction the fibres eliminated are shorter than half of the effective length.

It is the most regularly appearing length of the fibres in the representative sample. It is related to mean and median for curve distributions, as exhibited by fibre length, in the follwing way.

(Mode-Mean) = 3(Median-Mean)

where,

Median is the particular value of length above and below which exactly 50% of the fibres lie.

The complete sample analysis procedure can be divided into following steps:

The sample preparation is very important task during evaluation of fibre length. The representative sample is divided into 4 parts. Sixteen small tufts are taken from each corner at random of 20 mg. in size. Now all the tufts are reduced to half four times. These tufts are discarded, the fibres are parallelized and straightened alternatively with the help of left and right hand. Thus sixteen tufts from each corner is obtained. Now these sixteen tufts are combined together. Each set of sixteen tufts is combined separately. Thus four new tufts are obtained. Each new tuft is divided into four parts again. One tufts from each group is combined together. Thus sixteen tufts are converted into four new tufts. A quarter from each new tufts is taken and combined together. Now we get a final tufts of cotton fibres for testing. 20 mg. of cotton is taken for testing from final tufts. This method of sample preparation is known as

The representative sample of cotton is parallelized and the fibres are straightened by right and left hand alternatively. Many groups of fibre length are prepared. If we sort the fibre length groups manually, the sorting process gets very lengthy. A Shirley comb sorter apparatus is used to find the groups of various fibre length. These groups of fibre length are arranged on a velvet pad in descending order of fibre length. The one end of fibre length group is arranged in such a manner that this end touches the base line. All the groups of fibre length are arrange accurately on the base line. Extra care is taken during arranging the groups having very short fibre length. Finally we get the required fibres array of a representative sample as illustrated in the below figure:

NL' = (1/4) LL'

The above fibre's array is analysed as follows:

OA = Maximum fibre length

LL' = effective length of fibre

This parameter is determined with the help of digital fibrograph. The fbres of a representative sample are made parallel to each other. They are straightened up to optimum level. The the fibres in the specimen are distributed randomly. The initial scanning point is assumed as 100 ℅ fibres. Now the scanning is conducted at place where only 2.5 ℅ fibres of whole representative sample are present. Now the distance between initial point ( 100 ℅ fibres) and 2.5 ℅ fibres are recorded. This distance is termed as 2.5 ℅ span length of the fibres.

This parameter is determined with the help of digital fibrograph. The fbres of a representative sample are made parallel to each other. They are straightened up to optimum level. The the fibres in the specimen are distributed randomly. The initial scanning point is assumed as 100 ℅ fibres. Now the scanning is conducted at place where only 50 ℅ fibres of whole representative sample are present. Now the distance between initial scanning point ( 100 ℅ fibres) and 50 ℅ fibres are recorded. This distance is termed as 50 ℅ span length of the fibres.

Please see below graphic to understand the concept of span length of fibre.:

The South India Textile Research Association (SITRA) find the following equation based on observation and experience to find the Effective Length and Mean Length from the Span Lengths.

Effective length = (1.013 x 2.5% Span length) + 4.39

Mean length = ( 1.242 x 50% Span length )+ 9.78

Ring frame process and objectives of ring frame process

The " Fibre length" is a self explanatory word. It clearly tells us how long is the fibre. It is measured in inches or millimeters. It is the one of the most important characteristic of the cotton fibres.

Now we come on the topic "cotton fibre length. A cotton lint consists of many fibres. These fibres has different- different length individually. We can says many groups of lengths lie in the cotton lint. Since the cotton lint has many groups of fibre length, it gets very difficult to find exact fibre length of any cotton variety. The fibre length is the most important and critical characteristic of cotton fibre. It plays decisive role to determine the cost of any cotton variety. The fibre length directly influences many yarn parameters like the tensile strength, elongation, evenness and hairiness of the yarn to be spun. The spinner chooses correct fibre length to achieve desired yarn parameters to be spun. These yarn parameters directly affect the fabric to be woven.

It is very difficult to determine the exact value of the fibre length of cotton by using any apparatus. There are many terms used to express the fibre length of the cotton.

Some of the popular terms expressing the fibre length of cotton are given below:

Mean length.

Upper quartile.

Effective length.

Modal length.

2.5% span length.

50% span length.

**Mean length:**

**Mean length of cotton fibre is expressed in millimeters, centimeters or inches. " The arithmetic mean( average) of the length of all the fibres present in a representative sample of cotton lint is called mean length of a cotton fibre”. This quantity can be an average according to either number or weight.**

**Upper quartile length:**

It is that value of fibre length for which 3/4 of all the observed values in whole representative sample are lower, and 1/4 of all the observed value in whole representative sample are higher.

**Effective length:**

It is very difficult to define effective length technically. “ The upper quartile of a numerical length which is determined by making an arbitrary construction of a representative simple. This upper quartile length is called effective length of fibres”. In this arbitrary construction the fibres eliminated are shorter than half of the effective length.

**Modal length:**

It is the most regularly appearing length of the fibres in the representative sample. It is related to mean and median for curve distributions, as exhibited by fibre length, in the follwing way.

(Mode-Mean) = 3(Median-Mean)

where,

Median is the particular value of length above and below which exactly 50% of the fibres lie.

**COTTON SAMPLE ANALYSIS BY SHIRLEY COMB SORTER:**

The complete sample analysis procedure can be divided into following steps:

**Sample preparation:**

The sample preparation is very important task during evaluation of fibre length. The representative sample is divided into 4 parts. Sixteen small tufts are taken from each corner at random of 20 mg. in size. Now all the tufts are reduced to half four times. These tufts are discarded, the fibres are parallelized and straightened alternatively with the help of left and right hand. Thus sixteen tufts from each corner is obtained. Now these sixteen tufts are combined together. Each set of sixteen tufts is combined separately. Thus four new tufts are obtained. Each new tuft is divided into four parts again. One tufts from each group is combined together. Thus sixteen tufts are converted into four new tufts. A quarter from each new tufts is taken and combined together. Now we get a final tufts of cotton fibres for testing. 20 mg. of cotton is taken for testing from final tufts. This method of sample preparation is known as

*zoning technique.*

*PREPARATION OF FIBRES ARRAY:*

NL' = (1/4) LL'

**ANALYSIS OF ARRAY OF FIBRES:**

The above fibre's array is analysed as follows:

OA = Maximum fibre length

LL' = effective length of fibre

**CONCEPT OF SPAN LENGTH OF COTTON FIBRE:**

**2.5% Span length:**

This parameter is determined with the help of digital fibrograph. The fbres of a representative sample are made parallel to each other. They are straightened up to optimum level. The the fibres in the specimen are distributed randomly. The initial scanning point is assumed as 100 ℅ fibres. Now the scanning is conducted at place where only 2.5 ℅ fibres of whole representative sample are present. Now the distance between initial point ( 100 ℅ fibres) and 2.5 ℅ fibres are recorded. This distance is termed as 2.5 ℅ span length of the fibres.

**50 ℅ span length:**

This parameter is determined with the help of digital fibrograph. The fbres of a representative sample are made parallel to each other. They are straightened up to optimum level. The the fibres in the specimen are distributed randomly. The initial scanning point is assumed as 100 ℅ fibres. Now the scanning is conducted at place where only 50 ℅ fibres of whole representative sample are present. Now the distance between initial scanning point ( 100 ℅ fibres) and 50 ℅ fibres are recorded. This distance is termed as 50 ℅ span length of the fibres.

Please see below graphic to understand the concept of span length of fibre.:

The South India Textile Research Association (SITRA) find the following equation based on observation and experience to find the Effective Length and Mean Length from the Span Lengths.

Effective length = (1.013 x 2.5% Span length) + 4.39

Mean length = ( 1.242 x 50% Span length )+ 9.78

*You may also be interested in following articles:*Ring frame process and objectives of ring frame process

## No comments:

## Post a Comment